title: Localized and generalized simulated wear of resin composites.
abstract: A laboratory study was conducted to examine the wear of resin composite materials using both a localized and generalized wear simulation model. Twenty specimens each of seven resin composites (Esthet•X HD [HD], Filtek Supreme Ultra [SU], Herculite Ultra [HU], SonicFill [SF], Tetric EvoCeram Bulk Fill [TB], Venus Diamond [VD], and Z100 Restorative [Z]) were subjected to a wear challenge of 400,000 cycles for both localized and generalized wear in a Leinfelder-Suzuki wear simulator (Alabama machine). The materials were placed in custom cylinder-shaped stainless steel fixtures. A stainless steel ball bearing (r=2.387 mm) was used as the antagonist for localized wear, and a stainless steel, cylindrical antagonist with a flat tip was used for generalized wear. A water slurry of polymethylmethacrylate (PMMA) beads was used as the abrasive media. A noncontact profilometer (Proscan 2100) with Proscan software was used to digitize the surface contours of the pretest and posttest specimens. AnSur 3D software was used for wear assessment. For localized testing, maximum facet depth (μm) and volume loss (mm(3)) were used to compare the materials. The mean depth of the facet surface (μm) and volume loss (mm(3)) were used for comparison of the generalized wear specimens. A one-way analysis of variance (ANOVA) and Tukey post hoc test were used for data analysis of volume loss for both localized and generalized wear, maximum facet depth for localized wear, and mean depth of the facet for generalized wear. The results for localized wear simulation were as follows [mean (standard deviation)]: maximum facet depth (μm)--Z, 59.5 (14.7); HU, 99.3 (16.3); SU, 102.8 (13.8); HD, 110.2 (13.3); VD, 114.0 (10.3); TB, 125.5 (12.1); SF, 195.9 (16.9); volume loss (mm(3))--Z, 0.013 (0.002); SU, 0.026 (0.006); HU, 0.043 (0.008); VD, 0.057 (0.009); HD, 0.058 (0.014); TB, 0.061 (0.010); SF, 0.135 (0.024). Generalized wear simulation results were as follows: mean depth of facet (μm)--Z, 9.3 (3.4); SU, 12.8 (3.1); HU, 15.6 (3.2); TB, 19.2 (4.8); HD, 26.8 (6.5); VD, 29.1 (5.5); SF, 35.6 (8.4); volume loss (mm(3))--Z, 0.132 (0.049); SU, 0.0179 (0.042); HU, 0.224 (0.044); TB, 0.274 (0.065); HD, 0.386 (0.101); VD, 0.417 (0.076); SF, 0.505 (0.105). The ANOVA showed a significant difference among materials (p<0.001) for facet depth and volume loss for both localized and generalized wear. The post hoc test revealed differences (p<0.05) in localized and generalized wear values among the seven resin composites examined in this study. The findings provide valuable information regarding the relative wear characteristics of the materials in this study.
authors.forename: W W
authors.initials: WW
authors.lastname: Barkmeier
authors.forename: T
authors.initials: T
authors.lastname: Takamizawa
authors.forename: R L
authors.initials: RL
authors.lastname: Erickson
authors.forename: A
authors.initials: A
authors.lastname: Tsujimoto
authors.forename: M
authors.initials: M
authors.lastname: Latta
authors.forename: M
authors.initials: M
authors.lastname: Miyazaki
mesh_terms: D003188:Composite Resins / Q000592:standards / Q000627:therapeutic use*; D019554:Dental Restoration Wear; D006801:Humans; D008855:Microscopy, Electron, Scanning; D012822:Silicon Dioxide / Q000592:standards / Q000627:therapeutic use; D015040:Zirconium / Q000592:standards / Q000627:therapeutic use
chemical_list: D003188:Composite Resins; C466112:Esthet-X; C000590992:Filtek Supreme Ultra; C539358:Herculite Ultra; C000613185:SonicFill; C501891:Tetric EvoCeram; C488393:Venus (composite resin); C083568:Z100 composite resin; D012822:Silicon Dioxide; D015040:Zirconium